Materials Science and Engineering, 90 (1987) 307-315
Friction and Wear of Ion-beam-modified Ceramics for use in High Temperature Adiabatic Engines* WILLIAMWEIa, JAMES LANKFORDa and RAM KOSSOWSKYb aDepartrnent of Materials Sciences, Southwest Research Institute, San Antonio, TX (U.S.A.) bApplied Research Laboratory, State College, Pennsylvania State University, PA (U.S.A.)
(Received July 10, 1986)
A n experimental program has been conducted to investigate the friction and wear behavior o f ceramic materials being considered for use in high temperature adiabatic engines. Pin-on-disk-type tests were conducted in a simulated diesel environment at 800 °C using ceramic-ceramic couples made up o f SiC, TiC and TiC-Ni-Mo pins tested against Si3N 4 and partially stabilized ZrO 2 disk surfaces modified by ion beam mixing with cobalt, chromium, nickel or Ti-Ni. The coefficients o f friction for each couple were determined from these tests, and the amount o f wear was measured by profilometry o f the wear surfaces. Scanning electron microscopy, Auger electron spectroscopy and energy-dispersive spectroscopy were used to characterize the wear surfaces. The results o f these tests show that most non-ion-mixed ceramic-ceramic couples have relatively high wear rates and coefficients o f friction above about 0.25. Ion beam mixing o f disk material surfaces with Ti-Ni produced coefficients o f friction as low as O.06, values close to that for liquid-lubricated metal couples run at much lower temperatures. Surface modification with cobalt or nickel produced some promising results, while chromium did not improve the wear characteristics o f the disk materials. Auger analysis suggests that the formation o f lubricious oxide layers is responsible for the superior friction and wear behaviour o f the Ti-Ni-ion-implanted disks.
Improvements in low heat rejection engines and the development of a new generation of lighter, more energy-efficient engines and power systems has seen the increased application of ceramic materials to their construction, materials capable of withstanding the high operating temperatures and stresses required in such engines. The high temperature mechanical and chemical stability of many types of ceramic, most notably Si3Na and ZrO2, has made them candidates for use not only in stationary structural and insulating parts but also, with the recent consideration of allceramic engines, in moving parts [1, 2]. One of the major difficulties in the application of ceramics to the moving parts of high temperature engines has been the poor friction and wear performance of these materials. This problem is especially critical to applications such as cylinder liners and piston rings for high temperature adiabatic engines, or high temperature bearings in gas turbine engines, where engine design requirements include high temperatures, uncooled operation, and friction and wear properties of key parts comparable with those of conventional lubricated engines. In the last few years, numerous investigators have explored the friction and wear of ceramic-ceramic couples [3-5]. Although couples exhibiting minimum wear could be identified, wear was never negligible, and the unlubricated sliding friction coefficient 12F was usually discouragingly high, i.e. about 0.2 or more [3-11]. In fact, it has been generally concluded by some investigators that ceramic components will n o t be used unlubricated in sliding contact engine applications at either low [ 3] or elevated [ 4] temperatures.
*Paper presented at the International Conference
on SurfaceModification of Metals by Ion Beams, Kingston, Canada, July 7-11, 1986. 0025-5416/87/$3.50
© Elsevier Sequoia/Printed in The Netherlands
308 While this is a discouraging conclusion, especially in the light of the breakdown of conventional lubricants at elevated temperatures, certain observations made during these tests and other related investigations provide some insight as to how the wear properties of these materials might be improved to acceptable levels. In particular, the test environment has been shown to play a major role in the friction and wear behavior of ceramics. Coefficients of friction and wear rates have been found to be reduced when tests are conducted in oxidizing environments (air or water vapor) compared with tests conducted in inert environments (vacuum or inert gas) [ 12-14]. Surface analysis of the wear surfaces produced in these environments has shown that the formation of a thin oxide layer during testing in the oxidizing environments apparently provides a form of solid lubrication between the ceramic surfaces and is responsible for the improvement in the fricton and wear behavior of the ceramics tested [12-16]. An especially good example of this behavior is demonstrated by the titanium-based ceramics TiC and NiMo-bonded TiC cermet. When one of these materials is used as a member of a ceramicceramic couple, it has been shown that the coefficients of friction of these pairs often are reduced compared with those of other ceramic-ceramic combinations. This reduction is apparently the result of the formation and transfer of a TiO2 layer from the titaniumbased ceramic member to the other member of the couple [5, 17-22]. Oxygen does not necessarily have to be the lubrication-causing species for improved ceramic friction and wear behavior, however. Myristic acid, for instance, enhances surface plasticity and surface cracking during the sliding of steel on LiF , while the increased surface segregation of carbon as a graphite film on SiC has been shown to lead to a dramatic decrease in the coefficient of friction at temperatures above 800 °C . From the results of these studies, it appears that one promising direction toward the improvement of the friction and wear behavior of ceramics is to try to enhance these apparent self-lubricating properties. This could be achieved by a modification of the material surfaces which would, for example, enhance the growth of a lubricating oxide film. One such surface modification technique which
has shown initial success is the ion beam mixing of certain metals into ceramic surfaces and, in particular, into metals which are known to form stable continuous metal oxides and might induce this type of lubricating behavior [21, 22]. It has been shown that the surface ion mixing of a double layer of titanium and nickel in Si3N4 or partially stabilized ZrO 2 has improved the friction and wear properties of these materials in simulated diesel environments (at 800 °C) to levels approaching that of conventional lubricated engines run at lower temperatures . Auger electron spectroscopy (AES) indicates that the modified surface layer is apparently oxidized and provides a lubricating layer between the ceramic surfaces . The objective of this paper is to discuss further results on this preliminary investigation as well as to report on results of the ion beam mixing of other metals including cobalt, chromium and nickel.
2. EXPERIMENTAL PROCEDURE Details of the friction and wear experiments and subsequent surface analysis have been given in detail elsewhere [21, 22] and are summarized briefly here. Si3N4 and partially stabilized ZrO2 disks were surface modified by the ion beam mixing of cobalt, chromium, nickel or a Ti-Ni double layer. The choices of metal ions to be ion beam mixed were based on the results of unimplanted ceramic-ceramic tests (titanium and nickel) as discussed previously, and on work reported in the literature  which seemed to indicate possible lubricating properties for cobalt oxides and Cr203. The metals were vapor deposited on the ceramic disk substrates and then mixed into the surface by bombardment with argon ions. The argon ions were accelerated using a beam voltage of 140 keV, with a fluence of 1017 ions cm -2, and a flux of about 1012 ions cm -2 s -1. The thicknesses of the modified layers were estimated to be of the order of about 400 nm or less, based on subsequent Auger analysis. The modified disks, as well as unmodified disks, were tested in sliding contact in a threepin-on-disk arrangement where the pin materials were TiC or an Ni-Mo-bonded TiC cement. Tests were run in a simulated diesel environment or an inert argon atmosphere at 800 °C. The results of these tests are reported
primarily in terms of the coefficients of friction o f the various couples. Surface analysis of the wear surfaces of the pins and disks were c o n d u c t e d using scanning electron m i c r o s c o p y (SEM) and AES. The m o r p h o l o g y o f the wear surfaces was analyzed using SEM, while the chemistry of various features o f the wear surfaces was analyzed using AES. The results of these analyses were t h en correlated with the results of the mechanical friction and wear testing to provide a preliminary mechanism for the lubricating properties o f these modified surfaces.
3. R E S U L T S
appear to have no effect on the friction and wear behavior of the ceramic couples. The most promising pin-disk combinations include combinations 1 and 4 involving the Ti-Ni modification of Si3N 4 and partially stabilized ZrO2, where #F = 0.09, and combination 5 involving cobalt modification of partially stabilized ZrO2, where PF -~ 0.06. Comparison o f the combinations involving the Ti-Ni modification indicates t hat pin composition m ay also play a role in the friction and wear behavior of these materials. TiC appears to improve the coefficient of friction of the Ti-Ni-modified S i 3 N 4 disk, while the Ni-Mo-bonded TiC cermet appears to improve that of the Ti-Ni-modified Z r O 2. The latter is also the case for the cobalt-modified ZrO 2. However, there was no improvem e n t in the coefficient of friction for either of the cobalt-modified Si3N4 disks.
3.1. Friction and wear testing Results o f the friction and wear testing of the u n mo d if ied and modified ceramic-ceramic couples run in the simulated diesel environm e n t are summarized in Fig. 1 in terms of the steady state coefficient PF of friction. It is clear f r o m these results that, while the coeffi. . . . I O q cient o f friction f or pins run against u n m o d i . . . . I I I I L : i fied (bare) disks range above 0.2, surface o.~ I modification o f the disks by the ion beam o~, ~, ,' ,: O.G -(p~ns) I TiC I I mixing o f metals reduced the coefficients of ~ I :TiC i friction to values below 0.1 for certain specific .... o :KI62Be ; • 0.4 - K162B TIC K162B I cases, ~,&, : I KI6BBO I Values o f the coefficients of friction f or 02 I : 1 I I K1628O the modified disks are shown in Table I. The o., Cr ~I~ Co Bare ] Cr TIN1 CO metal ions showing the most promise for use ................ Olsk ~teria] Partlally Stabilized Zirconra Hot-Pressed Silicon Nitrtdes in the i m p r o v e m e n t of friction and wear behaviour by ion beam mixing appear to be TiFig. 1. S t e a d y s t a t e c o e f f i c i e n t o f f r i c t i o n a t 8 0 0 °C in Ni and cobalt, while c h r o m i u m and nickel a diesel e n v i r o n m e n t . t I
TABLE 1 C o e f f i c i e n t s o f f r i c t i o n o f p i n - m o d i f i e d disk c o m b i n a t i o n s t e s t e d in a diesel ( o x y g e n , n i t r o g e n , CO 2 a n d H 2 0 ) e n v i r o n m e n t at 8 0 0 °C Combination
D i s k a'b
1 2 3 4 5 6 7 8
Si3N 4 (Ti, Ni) Si3N 4 (Ti, Ni) Partially stabilized Partially stabilized Partially stabilized Partially stabilized Si3N 4 (Ni) Si3N 4 (Ni) ( t e s t e d
TiC TiC-5Ni-5Mo TiC TiC-5Ni-5Mo TiC-5Ni-5Mo TiC TiC TiC
ZrO 2 ZrO 2 ZrO 2 ZrO 2
(Ti, Ni) (Ti, Ni) (Co) (Co)
at r o o m t e m p e r a t u r e )
a Disk d i a m e t e r , 7.62 c m ; disk t h i c k n e s s , 0.95 cm. b T h e e l e m e n t s given in p a r e n t h e s e s are t h o s e ion b e a m m i x e d i n t o t h e surfaces of t h e disks. c Pin d i a m e t e r , 0 . 6 4 cm; pin l e n g t h , 1.27 cm.
0.09 0.22 0.25 0.09 0.06 > 0.25 0.14 > 0.28
Another major improvement resulting from the surface modification of the ceramic disks by ion beam mixing was the reduction in wear of the pinadisk combinations to the extent that in m a n y cases the a m o u n t of wear could n o t be measured either by mass change or by surface profilometry. For combinations 1-4 involving the Ti-Ni modification, and combinations 7 and 8 involving the nickel modification, the wear track on the disks was barely discernible by eye or in the electron microscope. The morphology of the wear process will be discussed in Section 3.2.
3.2. Surface analysis Typical results of the morphological and chemical analyses of the wear surfaces of the
Fig. 2. Wear surface of an Ni-Mo-bonded TiC cermet pin run against a Ti-Ni-modified partially stabilized ZrO 2 disk (diesel environment; 800 °C): (a) the arrow indicates the region magnified in (b); (b) magnification of (a). A indicates the transferred layer of nickel and titanium ;B indicates the original pin material. (Magnifications: (a) 40)( ; (b) 800X.)
modified ceramic couples are shown in Figs. 2-5. A typical wear surface from a pin is shown in Fig. 2, while wear surfaces from modified disks are shown in Figs. 3 and 4. Typical Auger elemental depth profiles from the modified disk surfaces are shown in Fig. 5. The pins from pin-disk combinations 1-6 showed a wear mark similar to that in Fig. 2(a) for the Ni-Mo-bonded cermet pin of combination 4. At a higher magnification (Fig. 2(b)), it appears that this mark is a layer of material which has transferred from the disk to the pin surface during sliding contact. AES analysis shows that this is indeed the case, the transfer layer containing nickel (and possibly titanium) transferred from the Ti-Ni modified disks [22 ], and cobalt transferred from the cobalt-modi-
Fig. 3. Wear surface of a Ti-Ni-modified partially stabilized ZrO 2 disk (diesel environment; 800 °C): (a) scanning electron micrograph; (b) Ti(387 eV) elemental map. The dark areas correspond to the exposed ZrO2 substrate shown by the arrows in (a) and (b).
Ni (848 eV) "
Fig. 4. Wear surface of a cobalt-modified partially stabilized ZrO 2 disk (diesel environment; 800 °C): (a) scanning electron micrograph; (b) Co(53 eV) elemental map. The light areas correspond to cobalt laminates left after friction and wear testing shown by the arrows in (a) and (b).
fied disks. Pins r u n against t h e n i c k e l - m o d i f i e d c o m b i n a t i o n s 7 a n d 8, as well as t h o s e r u n against c h r o m i u m - m o d i f i e d disks ( n o t given in T a b l e 1), s h o w n o such t r a n s f e r layer, ins t e a d e v i d e n c i n g a large a m o u n t o f d e l a m i n a t i o n - t y p e w e a r as d e s c r i b e d b y S u h [ 2 6 ] . A l t h o u g h m a n y o f t h e w e a r surfaces o n t h e m o d i f i e d disks w e r e d i f f i c u l t to o b s e r v e o p t i cally, scanning e l e c t r o n m i c r o g r a p h s s h o w t h a t w e a r o f t h e m o d i f i e d surfaces did i n d e e d o c c u r to v a r y i n g degrees. Figure 3 s h o w s a t y p i c a l w e a r surface f r o m a T i - N i - m o d i f i e d ZrO 2 disk, a n d Fig. 4 s h o w s a w e a r surface f r o m a c o b a l t - m o d i f i e d ZrO 2 disk. T h e previo u s s t u d y o n t h e T i - N i - m o d i f i e d disks indicated that the modified layer showed evidence o f d e l a m i n a t i o n w e a r [21, 2 6 ] , w i t h t h e disks
Sputter Time (mln)
Fig. 5. Typical elemental depth profiles taken (a) before and (b) after friction and wear testing of a Ti-Ni-modified Si3N 4 disk (diesel environment; 800 °C). Because of inhomogeneity of the preliminary mixing process and preferential sputtering, profiles are meant to show qualitative changes in the surfacemodified layer (see ref. 22).
w h i c h h a d higher c o e f f i c i e n t s o f f r i c t i o n ( c o m b i n a t i o n s 2 a n d 3) s h o w i n g larger a m o u n t s o f wear than those which had lower coefficients of friction. Elemental Auger maps of the wear surfaces such as t h a t in Fig. 3(b) s h o w e d t h a t d e l a m i n a t i o n o c c u r r e d along t h e m o d i f i e d layer-substrate interface. Auger depth profile analysis o f t h e m o d i f i e d layers i n d i c a t e d t h a t p o o r m i x i n g o f t h e m o d i f i e d layer w i t h t h e s u b s t r a t e m a y h a v e b e e n a cause f o r t h e del a m i n a t i o n o f t h e l a y e r (see Fig. 5(a)). H o w ever, s u b s e q u e n t m i x i n g a n d o x i d a t i o n o f t h e m o d i f i e d l a y e r at t h e high t e m p e r a t u r e s exp e c t e d at t h e c o n t a c t surfaces d u r i n g testing a p p a r e n t l y led to t h e i m p r o v e d f r i c t i o n a n d w e a r b e h a v i o r o b s e r v e d in t h e s i m u l a t e d diesel
312 environment, especially for the modified Si3N 4 disks (Fig. 5(b)). The results of the tests on cobalt-modified disks show behavior in some ways similar to that of the Ti-Ni-implanted disks. The cobaltmodified ZrO 2 disks have a low coefficient of friction when run against the TiC-Ni-Mo pin, and a much higher value when run against the TiC pin. However, unlike the Ti-Ni case, the SiaN 4 disks showed no improvement in the coefficient of friction when ion beam mixed with cobalt. Auger analysis of the cobalt-modified ZrO 2 disks and the corresponding pins indicates that cobalt transfers from the disk surface to the pins. Elemental depth profiles indicate that both the pin and the disk cobalt layers are oxidized, implying the presence of a lubricating cobalt oxide film analogous to the TiNi case. However, the physical characteristics of the wear tracks, especially for the low coefficient of friction disk, are disturbing. Both wear tracks show delamination of the cobalt layer, leaving exposed substrate. The wear track of the disk with a low coefficient of friction varies in width and a m o u n t of wear, ranging from the width of the pin with wear as heavy as that visible on the other three disks (see Fig. 4) to areas where the wear track is faint or almost non-existent (similar to Fig. 3). While it is thus possible that the ZrO 2 and Ni-Mo-bonded TiC results were influenced by the alignment of the pins and disk, the low coefficient of friction obtained indicates the transfer and possible lubricating effect of a cobalt oxide layer. AES analysis of the surface of the Ni-Mobonded TiC pin run against the cobalt-modified disk also shows the strong presence of nickel. This indicates that nickel segregates to the pin surface and may play a role in the friction and wear behavior of the ceramic couples. This also implies that nickel may have segregated from the pins in the Ti-Ni modification tests but would not be observable because of the nickel component of the modified layer. The results of tests involving the Ti-Ni- and the cobalt-modified disks suggest that nickel may play a particularly critical role in the friction and wear behavior of the ion-beammodified ceramics, either as a part of the modified layer or because of its presence in the pins. Therefore, two Si3N4 disks were ion beam modified with a layer of nickel and
tested in a diesel environment at 800 °C and at room temperature. The results of the friction and wear tests indicate that nickel improved the coefficient of friction of Si3N4, but n o t to the same degree as did the Ti-Ni modification or the cobalt in the ZrO 2 modification (see Table 1). Analysis of the wear surfaces of the disks and the pins showed that the nickel layer was completely worn off the disk and that no nickel transferred to the pins. The wear track shows cracking, especially near the edge of the crack, typical of the wear tracks of unmodified ceramics. The pin surfaces show clear signs of wear, as opposed to the adherence of a transfer layer seen in the Ti-Ni and cobalt cases. AES analysis of the unworn areas after testing shows, however, that the nickel layer was much better mixed into the substrate than in the two previous cases.
4. DISCUSSION The results of this investigation indicate that solid lubrication of ceramic materials at high temperatures is possible through the use of the technique of surface modification by ion beam mixing of oxide-forming metal ions. In order to optimize the conditions for the application of this technique to real systems, several factors must be considered. These include the characteristics and adhesive properties of the modified surface layer as governed by the operating environment, the ion-beammixing conditions, the choice of material substrates, the mechanism of lubrication by the modified layer (including its chemical state, the mechanical and structural properties and the possibility of its transfer from one material to the other) and the choice of the material to be run against the modified material. The adhesion at the ion-beam-modified layer-ceramic boundary is clearly important in the delamination-type wear observed, since this will govern the useful lifetime of the component. While this investigation was conducted on a screening basis, emphasizing shortterm tests to find promising ceramic-ceramic couples for immediate use in an experimental engine , the results of the analyses of the wear surfaces suggest that much longer hfetimes may be attainable through an optimization of the ion-beam-mixing conditions
313 an d /o r the choice and condition of the substrate materials and metal ions to be mixed. The previous study  showed t h a t the Ti-Ni modification appeared to mix the best in the SisN 4 substrate. While the a m o u n t of wear on the cobalt-modified disks was n o t satisfactory, the surface m o r p h o l o g y of the wear surface o f the cobalt-modified ZrO2 indicates t h a t the degree of initial surface roughness or initial microstructure in terms of grain size also may play an i m p o r t a n t role in the adhesion o f the modified layer. As can be seen in Fig. 6, traces of cobalt remain at pores, asperities and grain boundaries of the substrate surface, after argon sputtering has removed the main part of the modified surface. The results o f the tests c o n d u c t e d on disks modified only with nickel indicate that, while nickel alone does n o t improve the friction and wear behavior o f ceramics as well as ot her species, it may help to provide better bonding o f those species a n d / o r their lubricating oxides. F o r the Ti-Ni modification, TiO 2 appears to be responsible for the improved friction and wear behavior, but the nickel layer appears to be the bonding species which mixes into the substrate, especially for SisN 4. For the cobalt modification, segregation o f nickel f r o m the Ni-Mo-bonded TiC pin m a y be responsible for the adherence of the transferred cobalt to the pin surface at least temporarily, thus delaying the degradation of the friction and wear prop-
Fig. 6. Wear surface of the cobalt-modified ZrO 2 disk shown in Fig. 4 after sputter removal of most of the cobalt-modified layer. The remains of the cobalt layer are shown adhering to pores A, asperities B and grain boundaries C in the substrate surface.
erties caused by removal of the cobalt layer f r o m the disk surface. F u r t h e r work is required to determine the influence of nickel on the bonding a n d / o r friction and wear behavior o f ion ceramics. Also o f interest would be to det erm i ne those species which can be coupled with nickel in a modified layer to provide these beneficial results. For example, the ion beam mixing of c h r o m i u m alone apparently had no beneficial influence on the friction and wear behavior o f either SisN 4 or ZrO2, even when run against Ni-Mo-bonded TiC pins. The ion beam mixing o f c h r o m i u m with nickel m ay provide, however, an i m p r o v e m e n t similar to the Ti-Ni modification. The transfer of material or the f o r m a t i o n o f a surface oxide has been shown to be beneficial to the wear characteristics of the Ti-Nimodified ceramics, as well as to many ot her material systems in general [21, 22, 27, 28]. F r o m the results o f the present investigation, nickel appears to have been transferred f r o m the disks to the pins, or vice versa, as indicated by the results obtained f r o m the pins run against Ti-Ni- or cobalt-modified disks. Alt hough for the Ti-Ni modification, it is highly likely that titanium also transferred to the pins, it was n o t possible to determine definitely whether or n o t this was the case; a radioactive tracer technique would be useful for this determination for either nickel or titanium transfer. There appears to be no d o u b t t hat the modified and transferred layers had been oxidized and that this oxide cont ri but ed to t he i m provem ent in t he friction and wear properties of the modified ceramics. F u r t h e r investigations are under way to determine the characteristics of these oxides under the e x t r e m e conditions expect ed at the c o n t a c t surfaces in order to determine the mechanism of their lubricating effect. Characteristics such as oxide chemistry, mechanical or flow properties, and a m o r p h o u s v s . crystallographic structure would be expect ed to play i m p o r t a n t roles in the lubricating phenomenon. Some clues may be derived f r o m phase diagrams . The oxides of nickel show a strong dependence of their melting points on stoichiometry. Whereas NiO melts at close to 1600 °C, there is a sharp cont i nuous decrease in melting t e m p e r a t u r e with increase in the fraction of oxygen; Ni203 melts at less than 400 °C. It is quite plausible, therefore, t hat the tribological system of the sliding ceramics
314 was lubricated by a film of fluid NixOy where y / x is greater than unity. The relationships in
the Co-O system are less defined. It has been shown, however, that the stoichiometric CoO is the only form stable above 1000 °C. The higher oxygen compounds show significant instabilities at high temperatures where CoaO4, for example, dissociates at 900 °C. In contrast with the above, the oxides of chromium or titanium display high stabilities across the entire range of oxygen potentials. All titanium oxides are stable to at least 1600 °C. Similar observations hold for chromium oxides . Related to the material transfer question is the choice of material to be run against the modified ceramic. This choice would be made on the basis of not only the actual chemical processes discussed here but also the specific applications. The current investigation was conducted to screen ceramic-ceramic couples for use as cylinder liners and piston rings in high temperature adiabatic engines. As such, the material simulating the piston ring (the pin) would see constant sliding contact and thus would be susceptible to more wear than any particular point on the cylinder liner. Thus, for these tests, it was believed that the use of the harder modified ceramic which had some oxidizing capability (titanium) as the pin material would be more advantageous than modifying the pin surface. Other types of sliding application could benefit, however, from the use of modified ceramics for both members of the couple. From the previous investigation the choice of pin material played a confusing role in combinations 1-4 involving the Ti-Ni modification. Nickel was clearly transferred to all four pins , but the two pin materials had opposite effects with respect to disk material. The role of m o l y b d e n u m comes into question but, because of its volatility at high temperatures, it was not detected on any wear surfaces using AES. In contrast, nickel segregated from the Ni-Mo-bonded TiC pins may have played a role in the cobalt-modified disks.
5. CONCLUSIONS Pin-on-disk-type friction and wear tests have been conducted on a series of ceramicceramic couples in the unmodified state, and surface modified by ion beam mixing, in a
simulated environment typical of high temperature adiabatic diesel engines. Studies of the morphology and chemistry for the resulting wear surfaces have been conducted and correlated with the friction and wear behavior of these materials. It has been found that the surface modification of ceramics by the ion beam mixing of Ti-Ni or cobalt reduces the coefficient of friction (for certain specific pin-disk combinations) to levels falling in the upper end of • the range of values considered acceptable for conventional liquid-lubricated engines. In contrast, the ion beam mixing of chromium or nickel does not appear to have a beneficial effect on the friction and wear behavior of the materials tested. The improvement in friction and wear behavior of the ceramic couples modified with Ti-Ni and cobalt is apparently the result of the formation of a lubricating oxide of these species. Significant differences among all the material combinations examined, however, indicate that several factors must be investigated before this surface modification technique can be applied to real systems. These include (1) the characteristics and adhesion properties of the modified surface layer under operating conditions, (2) the effect of ion-beam-mixing conditions on the surface-modified layer and its ability to provide lubricating properties, (3) the mechanism of lubrication by the oxide layer and (4) the choice of materials and metals to be ion mixed for optimal lubricating behavior.
ACKNOWLEDGMENTS This work was conducted under a program sponsored by the U.S. Department of Energy and technically monitored by the Lewis Research Center, National Aeronautics and Space Administration, under Contract DEN3-352.
1 J.J. Burke, E. M. Lenoe and R. N. Katz (eds.), Proc. 2nd Int. Conf. on Ceramics for High Performance Applications, Newport, RI, March 2125, 19 77, Brook Hill Publishing, Chestnut Hill,
MA, 1978. 2 R. Kamo and W. Bryzik, Cumrnins/TACOM advanced adiabatic engine, in V. Danner (ed.), Adiabatic Engines: Worldwide Review, in SAE Spec.
5 6 7
8 9 10 11 12 13
14 15 16
Publ. SP-571, 1984, pp. 21-34 (Society of Automotive Engineers, Warrendale, PA). J. Breznak, E. Breval and N. H. Macmillan, J. Mater. Sci., 20 (1985) 4657. T. Shimachi, T. Murakami, T. Nakagaki, Y. Tsuya and K. Umeda, in V. Danner (ed.), Adiabatic Engines: Worldwide Review, in S A E Spec. Publ. SP-571, 1984, pp. 35-45 (Society of Automotive Engineers, Warrendale, PA). D. J. Boes, Proc. 22nd CCM, Society of Automotive Engineers, Warrendale, PA, 1984, p. 323. E. Rabinowicz, Friction and Wear o f Materials, Wiley, New York, 1965. K. Miyoshi and D. H. Buckley, in Tribology in the '80s, Vol. 1, in N A S A Conf. Publ. CP-2300, 1984, p. 291 (National Aeronautics and Space Administration). O. O. Adewoye and T. F. Page, Wear, 70 (1981) 37. D. W. Richerson, L. J. Lindberg, W. D. Carruthers and J. Dahn, Ceram. Eng. Sci. Proc., 2 (1981) 578. J. R. Smyth and D. W. Richerson, Ceram. Eng. Sci. Proc., 4 (1983) 663. M. B. Peterson and S. F. Murray, Met. Eng. Qt., 7 (2) (1967) 22. D.J. Barnes and B. D. Powell, Wear, 32 (1975) 195-202. P. Sutor, Tribology of silicon nitride and silicon nitride-steel sliding pairs, in F. D. Gac (ed.), Proc. 9th Annu. Conf. on Composites and Advanced Ceramic Materials, Cocoa Beach, FL, January 20-23, 1985, American Ceramic Society, Columbus, OH, 1985, pp. 460-469. T. E. Fischer and H. Tomizawa, Wear, 105 (1985) 29-45. R. P. Steijn, Wear, 7 (1964) 48-66. H. Shimura and Y. Tsuya, Effect of atmosphere on the wear rate of some ceramics and cements, Proc. Int. Conf. on the Wear o f Materials, St. Louis, MO, April 1977, American Society of
23 24 25
Mechanical Engineers, New York, 1977, pp. 452461. E. F. Finkin, S. J. Calabrese and M. B. Peterson, A S L E Prepr. 72LC-7C-2, 1972 (American Society of Lubrication Engineers). L. B. Sibley and C. M. Allen, Wear, 5 (1962) 312-329. Advanced Mechanical Technology Inc., Evaluation of improved materials for stationary diesel engines operating on residual and coal based fuels, Rep., 1980 (U.S. Department of Energy Contract DEAC-03-79ET15444). S. Gray, in F. D. Gac (ed.), Proc. 9th Annu. Conf. on Composites and Advanced Ceramic Materials, Cocoa Beach, FL, January 20-23, 1985, American Ceramic Society, Columbus, OH, 1985, pp. 965-975. J. Lankford, W. Wei and R. Kossowsky, Friction and wear behavior of ion beam modified ceramics, submitted to J. Mater. Sci. W. Wei and J. Lankford, Characterization of ion beam modified ceramic wear surfaces using Auger electron spectroscopy, submitted to J. Mater. Sci. D. H. Buckley, Ceram. Bull., 51 (1972) 884-905. K. Miyoshi and D. H. Buckley, Appl. Surf. Sci., 10 (1982) 357-376. W.J. Lackey and D. P. Stinton, Proc. 22nd Department o f Energy Contractors Coordinating Meeting, Society of Automotive Engineers, Warrendale, PA, 1984, p. 445. N.P. Suh, Wear, 25 (1973) 111. D. H. Buckley, Surface Effects in Adhesion, Friction, Wear, and Lubrication, Tribology Ser. 5, Elsevier, Amsterdam, 1984. I. L. Singer, Appl. Surf. Sci., 18 (1984) 28-62. Phase Diagrams for Ceramists, Vols. 3-5, American Society for Metals, Metals Park, OH, 19751980. R. P. Elliott, Constitution o f Binary Alloys, First Supplement, McGraw-Hill, New York, 1965, p. 327,